# stress-strain diagram - Home - KSU Faculty Member websites ``` Mechanical
Properties


Show relationship of stress
and strain using
experimental methods to
determine stress-strain
diagram of a specific
material
Discuss the behavior
described in the diagram for
commonly used engineering
materials
Discuss the mechanical properties and other test related to the development of
mechanics of materials
2
1.
2.
3.
4.
5.
6.
7.
8.
Tension and Compression Test
Stress-Strain Diagram
Stress-Strain Behavior of Ductile and Brittle
Materials
Hooke’s Law
Strain Energy
Poission’s Ratio
Shear Stress-Strain Diagram
*Failure of Materials Due to Creep and Fatigue
3



Strength of a material can only be determined
by experiment
One test used by engineers is the tension or
compression test
This test is used primarily to determine the
relationship between the average normal stress
and average normal strain in common
engineering materials, such as metals,
ceramics, polymers and composites
4
Performing the tension or compression test
 Specimen of material is made into “standard”
shape and size
 Before testing, 2 small punch marks identified
along specimen’s length
 Measurements are taken of both specimen’s
initial x-sectional area A0 and gauge-length
distance L0; between the two marks
 Seat the specimen into a testing machine shown
below
5
Performing the tension or compression test
 Seat the specimen into a testing machine shown
below
The machine will stretch specimen at slow
constant rate until breaking point
At frequent intervals during test, data is
recorded of the applied load P.
6
Performing the tension or compression test
 Elongation δ = L − L0 is measured using either a
caliper or an extensometer
 δ is used to calculate the normal strain in the
specimen
 Sometimes, strain can also be read directly using
an electrical-resistance strain gauge
7
A stress-strain diagram is obtained by plotting
the various values of the stress and
corresponding strain in the specimen
Conventional stress-strain diagram
 Using recorded data, we can determine nominal
or engineering stress by

σ=
P
A0
Assumption: Stress is constant over the x-section and throughout region between
gauge points
8
Conventional Stress-Strain Diagram
 Likewise, nominal or engineering strain is found
directly from strain gauge reading, or by
=
δ
L0
Assumption: Strain is constant throughout region between gauge points
By plotting σ (ordinate) against  (abscissa), we get a conventional stress-strain
diagram
9
Conventional stress-strain diagram
 Figure shows the characteristic stress-strain
diagram for steel, a commonly used material for
structural members and mechanical elements
10
Conventional stress-strain diagram
Elastic behavior.
A straight line
Stress is proportional to strain, i.e.,
linearly elastic
Upper stress limit, or proportional limit; σpl
If load is removed upon reaching elastic
shape
11
Conventional stress-strain diagram
Yielding.
Material deforms permanently; yielding;
plastic deformation
Yield stress, σY
Figure 3-4
Once yield point reached, specimen continues to elongate (strain) without any
Note figure not drawn to scale, otherwise induced strains is 10-40 times larger than
in elastic limit
Material is referred to as being perfectly plastic
12
Conventional stress-strain diagram
Strain hardening.
Ultimate stress, σu
While specimen is elongating, its xsectional area will decrease
Figure 3-4
Decrease in area is fairly uniform over entire
gauge length
13
Conventional stress-strain diagram
Necking.
At ultimate stress, x-sectional area
begins to decrease in a localized region
Figure 3-4
As a result, a constriction or “neck” tends to
form in this region as specimen elongates
further
Specimen finally breaks at fracture stress, σf
14
True stress-strain diagram
Instead of using original cross-sectional area and length, we can use the actual
cross-sectional area and length at the instant the load is measured
Values of stress and strain thus calculated are called true stress and true strain, and
a plot of their values is the true stress-strain diagram
15
True stress-strain diagram
In strain-hardening range, conventional σ- diagram shows specimen supporting
While true σ- diagram shows material to be sustaining increasing stress
16
True stress-strain diagram
Although both diagrams are different, most engineering design is done within
elastic range provided
1. Material is “stiff,” like most metals
2. Strain to elastic limit remains small
3. Error in using engineering values of σ and  is very small (0.1 %)
compared to true values
17
Ductile materials
 Defined as any material that can be subjected to
large strains before it ruptures, e.g., mild steel
 Such materials are used because it is capable of
absorbing shock or energy, and if before
deformation before failing
 Ductility of material is to report its percent
elongation or percent reduction in area at time of
fracture
18
Ductile materials
 Percent elongation is the specimen’s fracture
strain expressed as a percent
Percent elongation =
Lf − L0
(100%)
L0

Percent reduction in area is defined within
necking region as
Percent reduction in area =
A0 − Af
(100%)
A0
19
Ductile materials
 Most metals do not exhibit constant yielding
behavior beyond the elastic range, e.g.
aluminum
 It does not have well-defined yield point, thus it
is standard practice to define its yield strength
using a graphical procedure called the offset
method
20
Ductile materials
Offset method to determine yield strength
1.
2.
3.
Normally, a 0.2 % strain is chosen.
From this point on the  axis, a line
parallel to initial straight-line portion of
stress-strain diagram is drawn.
The point where this line intersects the
curve defines the yield strength.
21
Brittle Materials
 Material that exhibit little or no yielding before
failure are referred to as brittle materials, e.g.,
gray cast iron
 Brittle materials do not have a well-defined
tensile fracture stress, since appearance of
initial cracks in a specimen is quite random
22
Brittle Materials
 Instead, the average fracture stress from a set of
observed tests is generally reported
23
Most engineering materials exhibit a linear relationship between stress and strain
with the elastic region
Discovered by Robert Hooke in 1676 using springs, known as Hooke’s law
σ = E


E represents the constant of proportionality, also
called the modulus of elasticity or Young’s
modulus
E has units of stress, i.e., pascals, MPa or GPa.
24



As shown above, most
modulus of elasticity, Est = 200
GPa
Modulus of elasticity is a
mechanical property that
indicates the stiffness of a
material
Materials that are still have
large E values, while spongy
materials (vulcanized rubber)
have low values
25
IMPORTANT
 Modulus of elasticity E, can be used only if a
material has linear-elastic behavior.
 Also, if stress in material is greater than the
proportional limit, the stress-strain diagram
ceases to be a straight line and the equation is
not valid
26
Strain hardening
 If a specimen of ductile material (steel) is loaded
into the plastic region and then unloaded, elastic
strain is recovered as material returns to its
equilibrium state
 However, plastic strain remains, thus material is
subjected to a permanent set
27
Strain hardening
 Specimen loaded beyond yield point A to A’
 Inter-atomic forces have to be overcome to
elongate specimen elastically, these same
forces pull atoms back together when load is
removed
Since E is the same, slope of line O’A’ is
the same as line OA
28
Strain hardening
 Load reapplied, atoms will be displaced until
yielding occurs at or near A’, and stress-strain
diagram continues along same path as before
New stress-strain diagram has higher
yield point (A’), a result of strainhardening
Specimen has a greater elastic region and
less ductility
29
Strain hardening
energy may be lost
 Colored area between the curves represents lost
energy and is called mechanical hysteresis
It’s an important consideration when
selecting materials to serve as
dampers for vibrating structures and
equipment
30



energy is stored internally throughout its volume
Internal energy is also referred to as strain energy
Stress develops a force,
F = σ A = σ (x y)

Strain-energy density is strain energy per unit
volume of material
σ
∆U
u=
=
2
∆V
• If material behavior is linear elastic, Hooke’s law
applies,
σ σ
u=
2 
( )
σ2
=
2E
Modulus of resilience
 When stress reaches proportional limit, strainenergy-energy density is called modulus of
resilience
σpl pl σpl2
ur =
=
2E
2
• A material’s resilience represents
its ability to absorb energy
without any permanent damage
Modulus of toughness
 Modulus of toughness ut,
indicates the strain-energy
density of material before it
fractures
diagram is the modulus of
toughness
• Used for designing members that may be
• Higher ut is preferable as distortion is noticeable
before failure
Tension test for a steel alloy results in the stressstrain diagram below.
Calculate the
modulus of
elasticity and
the yield
strength based
on a 0.2%.
EXAMPLE 3.1 (SOLN)
Modulus of elasticity
Calculate the slope of initial straight-line portion of
the graph. Use magnified curve and scale shown in
light blue, line extends from O to A, with
coordinates (0.0016 mm, 345 MPa)
345 MPa
E=
0.0016 mm/mm
= 215 GPa
EXAMPLE 3.1 (SOLN)
Yield strength
At 0.2% strain, extrapolate line (dashed) parallel to
OA till it intersects stress-strain curve at A’
σYS = 469 MPa
EXAMPLE 3.1 (SOLN)
Ultimate stress
Defined at peak of graph, point B,
σu = 745.2 MPa
EXAMPLE 3.1 (SOLN)
Fracture stress
When specimen strained to maximum of f = 0.23
mm/mm, fractures occur at C.
Thus,
σf = 621 MPa


When body subjected to axial tensile force, it
elongates and contracts laterally
Similarly, it will contract and its sides expand
laterally when subjected to an axial compressive
force

Strains of the bar are:
δ
long =
L
δ’
lat =
r
• Early 1800s, S.D. Poisson realized that within
elastic range, ration of the two strains is a constant
value, since both are proportional.
lat
Poisson’s ratio, ν = − 
long




ν is unique for homogenous and isotropic material
Why negative sign? Longitudinal elongation
cause lateral contraction (-ve strain) and vice
versa
Lateral strain is the same in all lateral (radial)
directions
Poisson’s ratio is dimensionless, 0 ≤ ν ≤ 0.5
Bar is made of A-36 steel and behaves elastically.
Determine change in its length and change in
dimensions of its cross section after load is applied.
Normal stress in the bar is
P
σz =
= 16.0(106) Pa
A
From tables, Est = 200 GPa, strain in z-direction is
σz
z =
= 80(10−6) mm/mm
Est
Axial elongation of the bar is,
δz = zLz = [80(10−6)](1.5 m) = −25.6 μm/m
Using νst = 0.32, contraction strains in both x and y
directions are
x = y = −νstz = −0.32[80(10−6)] = −25.6 μm/m
Thus changes in dimensions of cross-section are
δx = xLx = −[25.6(10−6)](0.1 m) = −25.6 μm
δy = yLy = −[25.6(10−6)](0.05 m) = −1.28 μm


Use thin-tube specimens and subject it to
Record measurements of applied torque and
resulting angle of twist



Material will exhibit linear-elastic behavior till its
proportional limit, τpl
Strain-hardening continues till it reaches ultimate
shear stress, τu
Material loses shear strength till it fractures, at
stress of τf

Hooke’s law for shear
τ = Gγ
G is shear modulus of
elasticity or modulus of
rigidity
• G can be measured as slope of line on τ-γ diagram,
G = τpl/ γpl
• The three material constants E, ν, and G is related
by
E
G=
2(1 + ν)
Specimen of titanium alloy tested in
torsion &amp; shear stress-strain diagram
shown below.
Determine shear modulus G,
proportional limit, and ultimate shear
stress.
Also, determine the maximum
distance d that the top of the block
shown, could be displaced
horizontally if material behaves
elastically when acted upon by V.
Find magnitude of V necessary to
cause this displacement.
```